ORIGINAL ARTICLE DOI 10.1007/s10086-005-0787-7
M.I. Shams · T. Morooka · H. Yano (*)
Laboratory of Active Bio-based Materials, Research Institute for Sustainable Humanosphere, Kyoto University, Gokasho, Uji, Kyoto 611-0011, Japan
Tel. +81-774-38-3669; Fax +81-774-38-3600 e-mail: email@example.com
Md. Iftekhar Shams · Toshiro Morooka · Hiroyuki Yano
Compressive deformation of wood impregnated with low molecular weight
phenol formaldehyde (PF) resin V: effects of steam pretreatment
Received: July 22, 2005 / Accepted: November 16, 2005 / Published online: April 28, 2006
Abstract This study evaluated the potential of steam pre-treatment for making highly compressed phenol–formalde-hyde (PF) resin-impregnated wood at a low pressing pressure. Sawn veneers of Japanese cedar (Cryptomeria
japonica) were first subjected to saturated steam at different
steaming temperatures (140°–200°C), followed by impreg-nation with a 20% low molecular weight PF resin aqueous solution resulting in a weight gain of around 50%–55%. Four oven-dried treated veneers were laminated and com-pressed up to a pressing pressure of 1 MPa at a pressing temperature of 150°C and pressing speed of 5 mm/min, and the pressure was held for 30 min. Steam treatment, causing partial hydrolysis of hemicellulose, accelerated the com-pressibility of Japanese cedar in the PF resin-swollen condi-tion. As a consequence, a discernible increment in density was achieved at a pressing pressure of 1 MPa due to steam pretreatment between 140° and 200°C for 10 min. It was also found that even a short steaming time such as 2 min at 160°C is sufficient for obtaining appreciable compression of PF resin-impregnated wood. The density, Young’s modulus, and bending strength of steam-treated (200°C for 10 min) PF resin-impregnated wood composite reached 1.09 g/cm3
, 20 GPa, and 207 MPa, respectively. In contrast, the values of untreated PF resin-impregnated wood com-posite were 0.87 g/cm3
, 13 GPa, and 170 MPa, respectively.
Key words Compressed wood · Steam treatment · PF resin impregnation · Compressive deformation · Mechanical properties
Phenol–formaldehyde (PF) resin-impregnated compressed wood has been studied since the early half of the 20th century. This material, called Compreg, exhibits high strength, good dimensional stability, and high resistance to decay and termites.1,2
However, processing this material is severely curtailed by the need for high hot-pressing pres-sures in order to achieve its highly compressed condition, which results in a high-cost product thus having limited applications. Hence, the present authors developed a method to obtain highly compressed wood at low pressing pressure based on the analysis of the deforming behavior of PF resin-impregnated wood.3–6
First, we found that low molecular weight PF resin de-posited in the cell wall causes considerable softening, induc-ing the reduction of Young’s modulus perpendicular to the fiber direction, which results in cell wall collapse at low pressing pressure.3
Because of this collapse, PF resin-impregnated wood can be compressed significantly by the application of a slightly increasing or steady pressing pres-sure, which is in turn accompanied by an increment in mechanical properties.
The effects of processing parameters such as resin con-tent, preheating temperature, pressing temperature, and pressing speed were further investigated. It was demon-strated that by controlling these processing parameters properly, a highly compressed wood with high strength could be obtained at low pressing pressure.4
In addition, we studied species dependency in terms of the compressibility of wood after PF resin impregnation and identified that low-density wood species are potential candidates for the pro-duction of high-strength PF resin-impregnated wood at low pressing pressure.6
To obtain a further drastic deformation of PF resin-impregnated wood under compression, the effect of the removal of the matrix substances of the cell wall prior to resin impregnation was studied. It was found that a lignin-removing treatment using NaClO2 could significantly
fiber and is effective in utilizing collapse efficiently to obtain a high-strength resin-impregnated wood at a pressing pres-sure as low as 1 MPa.5
The above treatment is attractive; nevertheless it is com-plicated in processing. Furthermore, it is somewhat difficult to remove the harmful chemical, NaClO2, completely from
the treated wood, a factor that poses a major drawback in the application of this treatment.
For this reason, based on previous research,7–12
we fo-cused on steam treatment as an alternative pretreatment. An application of steam treatment for the production of dimensionally stable wood-based composites was devel-oped by Hsu et al.7
They found that steam treatment causes partial hydrolysis of the hemicellulose components, which greatly increases the compressibility of wood. The increase in compressibility by steam treatment is due to partial breakage of the matrix network cross-linked by lignin and carbohydrate components.10
Furthermore, it was found that the compressibility varied with steam temperature; at temperatures above 180°C wood shows significant de-formation.11
Thus, we have studied the potential of steam treatment in the range of 140°–200°C to enhance the com-pressibility of PF resin-impregnated wood.
Materials and methods
Sawn veneers of Japanese cedar (Cryptomeria japonica), with dimensions of 60 mm in the longitudinal direction (L), 40 mm in the tangential direction (T), and 1.5 mm in the radial direction (R), were cut in a series from a sapwood portion of a large block. Because density has a significant effect on the deformation behavior of PF resin-impregnated wood,6
veneers with a similar density were selected care-fully. Two series of wood samples were arranged: one for steaming temperature and the other for steaming time. Their ranges of air-dried density were 0.32–0.34 g/cm3 and 0.35–0.36 g/cm3
Veneers were subjected to saturated steam at different tem-peratures and times: 140°C, 160°C, 180°C, and 200°C for 10 min and 160°C for 2, 5, 10, 20, and 30 min (Table 1). The resultant steam pressures were 0.25 MPa for 140°C, 0.5 MPa for 160°C, 0.89 MPa for 180°C, and 1.4 MPa for 200°C. The weight loss was evaluated based on the oven-dried (105°C for 6 h) weight before and after steam treatment.
PF resin impregnation
An aqueous solution was prepared using a commercial low molecular weight PF resin with a molecular weight of about 300 (Gun-ei Chemical, PL 2771, pH 5.5, gelation time: 10 min at 150°C). Steam-treated and untreated veneers
were immersed in a 20% aqueous solution of PF resin for 3 days. The specimens were taken out of the solution and kept at ambient conditions for 3 days and vacuum dried at 50°C for 12 h, which is designated as oven-dried condition for PF resin-impregnated wood. The weight gain due to resin impregnation was evaluated based on the oven-dried weight before and after treatment.
Measurement of deformation behavior
Four plies of oven-dried veneer (without adhesive) were parallel laminated (approximately 6 mm in the radial direction) and compressed using an ordinary open system hot platens fixed to a universal testing machine (Instron 5500). The compression procedure was the same as de-scribed previously.3
Two compressed laminates were pro-duced for each condition. The hot pressing was carried out at 150°C at a pressing speed of 5 mm/min. After reaching a pressing pressure of 1 MPa, the crosshead movement was stopped and the pressure maintained for 30 min, hereafter called pressure holding. The relationship between pressing pressure and density was determined based on stress–strain curves.
Evaluation of mechanical properties
Two samples, 50 mm in the longitudinal direction by 8 mm in the tangential direction, were prepared from each plate. The Young’s modulus and bending strength were evaluated in the oven-dried condition by a three-point load-bending test at a crosshead speed of 5 mm/min and a test span of 40 mm, using an Instron 3365 universal testing machine. The values recorded were an average of the results of four samples.
Results and discussion
Table 1 shows the weight loss (WL, %) due to steam treat-ment and weight gain (WG, %) due to PF resin impregna-tion. The color of the samples became darker after steam Table 1. Effect of steam treatment on weight loss (WL) and weight gain (WG) due to phenol–formaldehyde (PF) resin impregnation
Temperature (°C) Time (min) WL (%) WG (%)
Control – – 52.2
140 10 1.8 59.2
160 2 0.7 54.1
160 5 0.9 51.4
160 10 2.5 53.3
160 20 3.6 53.5
160 30 5.0 52.6
180 10 4.8 57.7
treatment. The brownish color intensified with increases in the steaming temperature, especially at 200°C for 10 min. The weight loss tended to increase with increasing steaming temperature and time as reported previously.9,10
A maxi-mum weight loss of 7.4% was observed at 200°C for 10 min. The weight gain due to PF resin impregnation did not vary considerably, irrespective of steaming temperature and time as shown in Table 1.
Figure 1 displays the stress–strain curves of PF resin-impregnated wood as a function of steaming temperature. Steaming time was 10 min. In general, wood compressed in the radial direction, shows an elastic region followed by a long collapse-dominant region with roughly constant stress, leading to the final region of steeply rising stress called the postcollapse region. When solely steam-treated wood was compressed at oven-dried condition (St 160°C, OD), we could not detect any collapse deformation up to a pressing pressure of 1 MPa, showing to some extent the similar deformation behavior of untreated oven-dried Japanese cedar (C).
Hence, moisture was added to steam-treated wood, be-cause wood softens thermally to some extent in wet condi-tions due to the thermal softening of the matrix components such as hemicellulose and lignin.13 As shown in Fig. 1, steam-treated wood after adding moisture (St 160°C, AD) showed to a great extent deformation when compared with the oven-dried condition. It started collapsing at up to 1 MPa, although it was difficult to point out the exact posi-tion of the collapse-initiating stress. This behavior corre-sponds to the previous findings that steam treatment is
effective to enhance the compressibility of wood.7,10 How-ever, as clearly demonstrated in Fig. 1, the behavior is not as distinct as that of oven-dried PF resin-impregnated wood (PF resin impregnated) especially in the collapse-dominant region.
The collapse-initiating stress was dramatically reduced by the combination of steam treatment and PF resin im-pregnation (St + PF). Steam treatment at a relatively lower temperature such as 140°C prior to PF resin impregnation reduced the collapse-initiating stress from 0.8 MPa of solely PF resin-impregnated wood to 0.3 MPa. The collapse-initiating stress remained constant over the range of tem-peratures from 140° to 180°C despite the decomposition of the cell wall polymers demonstrated by increased weight loss, although a long collapse-dominant region with roughly constant stress was distinct at 180°C. The collapse-initiating stress decreased with increasing steaming temperature from 180°C to 200°C, and it was noted that cell wall collapse started at 0.2 MPa when steam treatment was performed at 200°C for 10 min.
The compressibility of steam-treated PF resin-impregnated wood was further studied at 160°C as a func-tion of steaming time. As shown in Fig. 2, the stress required to compress PF resin-impregnated wood was greatly influ-enced by the steaming time. Interestingly, at a steaming treatment time of 2 min, which resulted in a small weight loss of 0.7%, the collapse-initiating stress reduced from 0.8 to 0.5 MPa. As steaming time increased, the collapse tended to start at lower stress. At a steaming time of 30 min and a weight loss of 5.0%, the collapse-initiating stress fell to 0.3 MPa, which is comparable with that for 180°C for 10 min having a weight loss of 4.8%. This implies that the collapse-initiating stress closely corresponded to the degree of de-composition of the cell wall polymers as indicated by weight loss.
0.0 0.2 0.4 0.6 0.8 1.0
0 0.1 0.2 0.3 0.4 0.5 0.6 0.7
St 160ºC, OD
PF resin impregnated
St 140ºC + PF
St 160ºC + PF
St 180ºC + PF St 160ºC, AD
St 200ºC + PF C
Fig. 1. Stress–strain curves of oven-dried phenol–formaldehyde (PF) resin-impregnated wood as a function of steaming temperature at a pressing temperature of 150°C and pressing speed of 5 mm/min. C, control (oven-dried untreated Japanese cedar); St, steam temperature;
PF, phenol-formaldehyde resin impregnated; OD, oven-dried
condi-tion; AD, air-dried condition. Steaming time was 10 min
0.0 0.2 0.4 0.6 0.8 1.0
0 0.1 0.2 0.3 0.4 0.5 0.6 0.7
The decomposition of cell wall polymers due to steam treatment has been studied extensively.14–18
The chemical structure of wood differs among species, especially between softwood and hardwood; thus, the decomposing manner of cell wall polymers differs among wood species. In the case of Japanese cedar, Higashihara et al.15
reported that the hemicellulose decreased remarkably by steam treatment at 180°C for 60 min whilst the lignin of Japanese cedar appar-ently did not change. Dwianto et al.12
considered that steam-ing up to 200°C for 60 min induces the decomposition of hemicellulose and is probably accompanied by slight de-composition of lignin. Thus, it appears that for up to 180°C for 10 min or 160°C for 30 min, the change in chemical components of Japanese cedar is attributable to the de-composition of hemicellulose. Thus, it can be said that the decomposition of hemicellulose due to steam treatment ac-celerates the compressibility of Japanese cedar in the PF resin-swollen condition.
Pressing pressure–density relationships
A more practical expression of the stress–strain relationship is the pressing pressure–density relationship, because den-sity is an important parameter in determining the change in mechanical properties of resin-impregnated compressed wood.3
The pressing pressure–density relationship was evaluated based on the final density of the compressed samples and thickness changes during compression. The relationship is depicted in Fig. 3 as a function of steaming temperature. There was a drastic change in density due to steam treatment. A steaming temperature of 140°C caused a weight loss of 1.8% and enabled a discernible increment of density: about 20% higher than in the untreated condi-tion (Un) at 1 MPa. The difference can be explained by the
difference of collapse-initiating stress shown in Fig. 1. The density at 1 MPa did not differ between 140° and 180°C, as could be expected from Fig. 1. However, the density showed a marked increment from 180° to 200°C, attaining a density of 0.98 g/cm3
at 1 MPa, which is about 1.4 times higher than that of untreated PF resin-impregnated wood (Un).
When the pressing pressure–density relationship was evaluated as a function of steaming time at 160°C, it was observed that the density increased with increasing steam-ing time and attained around 0.93 g/cm3
when the steaming time was 30 min. Furthermore, it is interesting to show that the density of PF resin-impregnated wood reached a density of 0.8 g/cm3
at a short steaming time such as 2 min, about 15% higher than that of untreated PF resin-impregnated wood (Un).
The pressing pressure–density relationship of steam-treated resin-impregnated wood is compared in Fig. 3 with those of NaClO2-treated (a lignin removal treatment)
The weight loss due to NaClO2
treatment was 21%, and the weight gain due to PF resin impregnation for NaClO2-treated wood was 60%. As
there was a significant difference in compressibility between air-dried and oven-dried condi-tions for NaClO2-treated PF resin-impregnated wood. The
density of NaClO2-treated resin-impregnated wood was
for the oven-dried condition (NaClO2 treatment,
OD) at a pressing pressure of 1 MPa. After adding moisture of 10%–11% to the NaClO2-treated resin-impregnated
wood (NaClO2 treatment, AD), the density reached 1.0 g/
. This is similar to the density attained by oven-dried steam-treated resin-impregnated wood (200°C). It is worth mentioning that the decomposition of hemicellulose is as effective in increasing the compressibility of PF resin-impregnated wood as is the removal of lignin. Based on the chemical analysis of Higashihara et al.,15
it is believed that a large amount of low molecular weight substances derived from decomposition of hemicellulose still remain in the cell wall after steaming. From these facts, it may be speculated that the decomposed hemicellulose maintained in the cell wall acts as a plasticizer in combination with the low mo-lecular weight PF resin, and reduces the Young’s modulus of the cell wall. It is thus recommended that steam treat-ment can be substituted for chemical treattreat-ment in the fabri-cation of highly compressed PF resin-impregnated wood, because steam treatment is much easier to perform than NaClO2 treatment and is harmless to humans.
Mechanical properties of compressed wood
Figure 4 shows the density and mechanical properties of steam-treated PF resin-impregnated wood after pressure holding for 30 min at 1 MPa. The steaming time was 10 min. The density of PF resin-impregnated wood increased during pressure holding. For example, untreated PF resin-impregnated wood (Un) showed an increment of density from 0.70 to 0.87 g/cm3
, and steam-treated (140°C) PF resin-impregnated wood increased from 0.85 to 1.03 g/cm3
0.4 0.5 0.6 0.7 0.8 0.9 1.0
0.0 0.2 0.4 0.6 0.8 1.0
Pressing pressure, MPa
NaClO2 treatment, OD
140°C 160°C 180°C 200°C
NaClO2 treatment, AD
Fig. 3. Changes of density of PF resin-impregnated wood as a function of steaming temperature and comparison with NaClO2 treatment.
Pressure holding causing creep deformation of the cell wall is effective for the further densification of PF resin-impreg-nated wood. Furthermore, it was observed that within 1 min of pressure holding, the density increased considerably irre-spective of the steaming temperature and afterward became stabilized, as reported previously.3
The Young’s modulus and bending strength of PF resimpregnated wood at a pressing pressure of 1 MPa in-creased due to steam pretreatment, and attained 20 GPa and 207 MPa, respectively, when the steaming treatment was 200°C and 10 min as shown in Fig. 4. This improvement is mainly attributable to the increased compressibility by the combination of steam treatment and PF resin impregna-tion. Furthermore, the specific Young’s modulus (the ratio of Young’s modulus to the specific gravity) was found to
increase due to steam pretreatment. This increment is likely to cause the increase of the volume fraction of cellulose microfibril. The specific bending strength (the ratio of bend-ing strength to the specific gravity) did not show any significant decrease, even when pretreated at a high steam-ing temperature such as 200°C. Thus, it can be concluded that steam treatment prior to PF resin impregnation and pressure holding is desirable in obtaining high-strength PF resin-impregnated compressed wood at low pressing pressure.
Because the Young’s modulus and bending strength of untreated oven-dried Japanese cedar in this study were 5.0 GPa and 40.8 MPa, respectively, the mechanical pro-perties of Japanese cedar improved four- to fivefold by the combination of steam pretreatment, PF resin impregnation, and hot pressing at 1 MPa. Considering that 1 MPa is a typical pressing pressure used for ordinary plywood and laminated veneer lumber (LVL) production, our finding indicates that when steam-treated PF resin-impregnated Japanese cedar veneers are laminated on both surfaces of stacked untreated veneers prior to hot pressing, high-strength plywood or LVL having dimensionally stabilized surfaces and a moderate specific gravity can be obtained by one-shot hot pressing. The application of this promising technique in making high-strength plywood and LVL is underway and will be reported in a future article.
We have demonstrated that steam treatment prior to PF resin impregnation enables marked deformation of PF resin-impregnated wood at low pressing pressure. The den-sity of steam-treated PF resin-impregnated compressed wood was much higher than that of NaClO2-treated PF
resin-impregnated wood when compared in their oven-dried conditions. It is recommended that steam treatment be substituted for chemical treatment in the fabrication of highly compressed PF resin-impregnated wood. Steam treatment is much easier to perform than NaClO2 treatment
and is harmless to humans. Such treated wood elements present a promising surface material in the manufacture of sandwich panels, giving high strength and dimensional sta-bilization with a moderate specific gravity using a one-shot application.
Acknowledgments The authors thank Gun-ei Chemical Industry Ltd. for supplying low molecular weight phenol–formaldehyde resin. The first author is indebted to the Ministry of Education, Culture, Sports, Science, and Technology, Government of Japan, for support provided by a Grant-in-Aid.
1. Stamm AJ (1964) Wood and cellulose science. Ronald, New York, pp 343–358
2. Stamm AJ, Bachelor RH (1960) Decay resistance and dimensional stability of five modified woods. Forest Prod J 10:22–26
0 5 10 15 20 25
Un 140 160 180 200
0 50 100 150 200 250
200 180 160 140 Un 0.0
0.2 0.4 0.6 0.8 1.0 1.2
Un 140 160 180 200
Fig. 4a–c. Effects of steam treatment on a density, b Young’s modulus, and c bending strength of PF resin-impregnated compressed wood. All samples were compressed at 1 MPa with a pressure holding of 30 min.
Un refers to PF resin-impregnated wood. The numbers are the
steam-ing temperatures (°C). Steamsteam-ing time was 10 min. Bars represent stan-dard deviations
3. Shams MI, Yano H, Endou K (2004) Compressive deformation of wood impregnated with low molecular weight phenol formalde-hyde (PF) resin I. Effects of pressing pressure and pressure hold-ing. J Wood Sci 50:337–342
4. Shams MI, Yano H (2004) Compressive deformation of wood im-pregnated with low molecular weight phenol formaldehyde (PF) resin II. Effects of processing parameters. J Wood Sci 50:343–350 5. Shams MI, Yano H, Endou K (2005) Compressive deformation of wood impregnated with low molecular weight phenol formalde-hyde (PF) resin III. Effects of sodium chlorite treatment. J Wood Sci 51:234–238
6. Shams MI, Kagemori N, Yano H (2006) Compressive deformation of wood impregnated with low molecular weight phenol formalde-hyde (PF) resin IV: species dependency. J Wood Sci 52:179–183 7. Hsu WE, Schwald W, Schwald J, Shields A (1988) Chemical and
physical changes required for producing dimensionally stable wood-based composites. Part 1. Steam pretreatment. Wood Sci Technol 22:281–289
8. Inoue M, Norimoto M, Tanahahi M, Rowell RM (1993) Steam or heat fixation of compressed wood. Wood Fiber Sci 25:224–235 9. Sekino N, Inoue M, Irle M, Adcock T (1999) The mechanisms
behind the improved dimensional stability of particleboards made from steam-pretreated particles. Holzforschung 53:435–440 10. Inoue M, Sekino N, Morooka T, Norimoto M (1996) Dimensional
stabilization of wood composites by steaming. Part 1. Fixation of compressed wood by pre-steaming. Proceedings of the 3rd Pacific Rim Bio-based Composites Symposium, Kyoto, Japan, pp 240–248
11. Irle M, Adcock T, Sekino N (1998) The rheological behavior and dimensional stability of steam pretreated particles. Proceedings of the 2nd European Panel Products Symposium, Llandudno, UK, pp 24–29
12. Dwianto W, Morooka T, Norimoto M, Kitajima T (1999) Stress relaxation of Sugi (Cryptomeria japonica D. Don) wood in radial compression under high temperature steam. Holzforschung 53: 541–546
13. Goring DAI (1963) Thermal softening of lignin, hemicellulose and cellulose. Pulp Pap Canada 64:517–527
14. Lawther JM, Sun R, Banks WB (1996) Effect of steam treatment on the chemical composition of wheat straw. Holzforschung 50:365–371
15. Higashihara T, Morooka T, Hirosawa S, Norimoto M (2004) The relationship between change of chemical components and permanent fixation of compressed wood by steaming or heating (in Japanese). Mokuzai Gakkaishi 50:159–167
16. Tanahashi M, Tamabuchi K, Goto T, Aoki T, Karina M, Higuchi T (1988) Characterization of steam-exploded wood II: chemical changes of wood components by steam explosion. Wood Res 75:1– 12
17. Widyorini R, Xu J, Watanabe T, Kawai S (2005) Chemical changes in steam-pressed kenaf core binderless particleboard. J Wood Sci 51:26–32